#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/05/4500568.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4500568
loop_
_publ_author_name
'Liu, Hai-Yan'
'Wu, Hua'
'Yang, Jin'
'Liu, Ying-Ying'
'Ma, Jian-Fang'
'Bai, Hong-Ye'
_publ_section_title
;
 Solvothermal Assembly of a Series of Organic--Inorganic Hybrid Materials
 Constructed from Keggin Polyoxometalate Clusters and Copper(I)--Organic
 Frameworks
;
_journal_issue                   5
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              1786
_journal_paper_doi               10.1021/cg1017246
_journal_volume                  11
_journal_year                    2011
_chemical_formula_moiety         'C24 H35 Cu4 Mo12 N8 O41.50 P'
_chemical_formula_sum            'C24 H35 Cu4 Mo12 N8 O41.5 P'
_chemical_formula_weight         2536.01
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 112.811(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   23.4725(7)
_cell_length_b                   12.0745(3)
_cell_length_c                   23.1288(7)
_cell_measurement_reflns_used    6164
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.4
_cell_measurement_theta_min      1.9
_cell_volume                     6042.4(3)
_computing_cell_refinement       CrysAlis
_computing_data_collection       'CrysAlis (Oxford Diffraction, 2006)'
_computing_data_reduction        CrysAlis
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Oxford Diffraction Gemini R Ultra'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0445
_diffrn_reflns_av_sigmaI/netI    0.0879
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            15276
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         1.91
_exptl_absorpt_coefficient_mu    3.901
_exptl_absorpt_correction_T_max  0.67
_exptl_absorpt_correction_T_min  0.52
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlis (Oxford Diffraction, 2006)
;
_exptl_crystal_colour            blacl
_exptl_crystal_density_diffrn    2.788
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             4808
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.966
_refine_diff_density_min         -0.832
_refine_diff_density_rms         0.161
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.859
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     427
_refine_ls_number_reflns         6164
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.859
_refine_ls_R_factor_all          0.0920
_refine_ls_R_factor_gt           0.0416
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0475P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0867
_refine_ls_wR_factor_ref         0.0964
_reflns_number_gt                3413
_reflns_number_total             6164
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            cg1017246_si_002.cif
_cod_data_source_block           5
_cod_original_sg_symbol_Hall     '-C 2yc '
_cod_original_sg_symbol_H-M      'C 2/c '
_cod_original_formula_sum        'C24 H35 Cu4 Mo12 N8 O41.50 P'
_cod_database_code               4500568
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu 0.80327(4) -0.17035(9) 0.38506(4) 0.0454(3) Uani 1 1 d .
Cu2 Cu 1.05729(5) -0.31258(11) 0.62271(5) 0.0621(4) Uani 1 1 d .
Mo1 Mo 0.61113(3) 0.14151(6) 0.38516(3) 0.03455(18) Uani 1 1 d .
Mo2 Mo 0.71239(3) 0.30367(6) 0.33774(3) 0.03524(18) Uani 1 1 d .
Mo3 Mo 0.62389(3) 0.43072(6) 0.41648(3) 0.03523(18) Uani 1 1 d .
Mo4 Mo 0.65034(3) 0.08234(6) 0.54704(3) 0.03937(19) Uani 1 1 d .
Mo5 Mo 0.73679(4) -0.03746(6) 0.46809(3) 0.0409(2) Uani 1 1 d .
Mo6 Mo 0.66096(3) 0.37366(6) 0.57818(3) 0.04050(19) Uani 1 1 d .
C1 C 0.8778(4) -0.2371(7) 0.5068(3) 0.044(2) Uani 1 1 d .
H1 H 0.8403 -0.2318 0.5115 0.053 Uiso 1 1 calc R
C2 C 0.9296(4) -0.2675(6) 0.5579(3) 0.0375(19) Uani 1 1 d .
C3 C 0.9278(4) -0.2883(7) 0.6213(3) 0.055(2) Uani 1 1 d .
H3A H 0.9682 -0.3096 0.6504 0.082 Uiso 1 1 calc R
H3B H 0.8989 -0.3466 0.6181 0.082 Uiso 1 1 calc R
H3C H 0.9151 -0.2220 0.6359 0.082 Uiso 1 1 calc R
C4 C 0.9838(4) -0.2560(7) 0.4946(4) 0.048(2) Uani 1 1 d .
H4 H 1.0207 -0.2645 0.4892 0.058 Uiso 1 1 calc R
C5 C 0.9327(4) -0.2225(7) 0.4439(3) 0.042(2) Uani 1 1 d .
C6 C 0.9364(4) -0.1948(8) 0.3832(3) 0.059(3) Uani 1 1 d .
H6A H 0.8963 -0.1731 0.3537 0.088 Uiso 1 1 calc R
H6B H 0.9503 -0.2584 0.3674 0.088 Uiso 1 1 calc R
H6C H 0.9650 -0.1349 0.3890 0.088 Uiso 1 1 calc R
C7 C 1.1071(4) -0.5284(8) 0.7083(4) 0.068(3) Uani 1 1 d .
H7A H 1.0717 -0.5113 0.6711 0.101 Uiso 1 1 calc R
H7B H 1.0938 -0.5606 0.7390 0.101 Uiso 1 1 calc R
H7C H 1.1331 -0.5798 0.6984 0.101 Uiso 1 1 calc R
C8 C 1.1423(3) -0.4251(7) 0.7341(3) 0.040(2) Uani 1 1 d .
C9 C 1.1956(3) -0.4232(7) 0.7884(3) 0.040(2) Uani 1 1 d .
H9 H 1.2102 -0.4900 0.8089 0.048 Uiso 1 1 calc R
C10 C 1.2028(4) -0.2353(7) 0.7853(3) 0.039(2) Uani 1 1 d .
C11 C 1.2345(5) -0.1292(8) 0.8136(4) 0.078(3) Uani 1 1 d .
H11A H 1.2706 -0.1452 0.8504 0.117 Uiso 1 1 calc R
H11B H 1.2068 -0.0837 0.8248 0.117 Uiso 1 1 calc R
H11C H 1.2463 -0.0907 0.7836 0.117 Uiso 1 1 calc R
C12 C 1.1498(4) -0.2347(8) 0.7313(4) 0.054(2) Uani 1 1 d .
H12 H 1.1340 -0.1673 0.7123 0.065 Uiso 1 1 calc R
N1 N 0.8792(3) -0.2149(5) 0.4512(3) 0.0348(15) Uani 1 1 d .
N2 N 0.9837(3) -0.2771(5) 0.5516(3) 0.0450(17) Uani 1 1 d .
N3 N 1.1205(3) -0.3290(7) 0.7053(3) 0.0476(18) Uani 1 1 d .
N4 N 1.2271(3) -0.3313(5) 0.8130(2) 0.0330(15) Uani 1 1 d .
O1 O 0.7961(4) 0.3505(7) 0.5200(3) 0.024(2) Uani 0.50 1 d P
O2 O 0.7875(4) 0.1467(7) 0.4973(4) 0.027(2) Uani 0.50 1 d P
O3 O 0.7744(4) 0.2660(7) 0.4473(4) 0.028(2) Uani 0.50 1 d P
O4 O 0.6990(4) 0.2743(7) 0.4391(4) 0.024(2) Uani 0.50 1 d P
O5 O 0.7701(3) 0.1878(5) 0.3525(3) 0.075(2) Uani 1 1 d .
O6 O 0.7790(3) 0.4018(5) 0.3771(3) 0.081(2) Uani 1 1 d .
O7 O 0.6937(3) 0.3321(5) 0.2625(2) 0.0584(18) Uani 1 1 d .
O8 O 0.6610(3) 0.4110(5) 0.3570(3) 0.0580(17) Uani 1 1 d .
O9 O 0.5869(3) 0.2894(4) 0.3923(3) 0.0552(16) Uani 1 1 d .
O10 O 0.5647(3) 0.5143(5) 0.3782(3) 0.0685(19) Uani 1 1 d .
O11 O 0.6884(3) 0.5316(5) 0.4594(2) 0.070(2) Uani 1 1 d .
O12 O 0.6522(3) 0.1973(4) 0.3349(3) 0.0589(17) Uani 1 1 d .
O13 O 0.6138(3) 0.4082(6) 0.4949(2) 0.079(2) Uani 1 1 d .
O14 O 0.6196(3) 0.4318(5) 0.6140(2) 0.0599(17) Uani 1 1 d .
O15 O 0.6275(3) 0.2293(5) 0.5638(3) 0.070(2) Uani 1 1 d .
O16 O 0.6019(3) 0.1078(6) 0.4613(3) 0.087(3) Uani 1 1 d .
O17 O 0.6941(3) -0.0270(6) 0.5224(2) 0.076(2) Uani 1 1 d .
O18 O 0.6665(3) 0.0183(6) 0.4029(3) 0.084(2) Uani 1 1 d .
O19 O 0.7320(2) -0.1718(4) 0.4499(2) 0.0369(13) Uani 1 1 d .
O20 O 0.7843(3) 0.0090(5) 0.4206(2) 0.0657(19) Uani 1 1 d .
O21 O 0.5470(3) 0.0892(5) 0.3325(3) 0.0616(17) Uani 1 1 d .
O22 O 0.6032(3) 0.0072(4) 0.5685(2) 0.0487(15) Uani 1 1 d .
P1 P 0.7500 0.2500 0.5000 0.0197(5) Uani 1 2 d S
O1W O 1.0556(9) -0.0370(16) 0.7368(8) 0.133(7) Uiso 0.50 1 d P
O2W O 1.0000 0.160(3) 0.7500 0.151(11) Uiso 0.50 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N4 Cu1 N1 164.0(3) 8_445 .
N4 Cu1 O20 93.1(2) 8_445 .
N1 Cu1 O20 102.5(2) . .
N2 Cu2 N3 165.5(3) . .
O21 Mo1 O12 102.7(3) . .
O21 Mo1 O16 101.7(3) . .
O12 Mo1 O16 155.7(3) . .
O21 Mo1 O9 101.8(3) . .
O12 Mo1 O9 87.7(2) . .
O16 Mo1 O9 88.6(3) . .
O21 Mo1 O18 102.1(3) . .
O12 Mo1 O18 86.7(3) . .
O16 Mo1 O18 87.0(2) . .
O9 Mo1 O18 156.0(3) . .
O21 Mo1 O1 157.9(3) . 7_656
O12 Mo1 O1 92.8(3) . 7_656
O16 Mo1 O1 63.5(3) . 7_656
O9 Mo1 O1 94.5(3) . 7_656
O18 Mo1 O1 62.6(3) . 7_656
O7 Mo2 O5 102.9(3) . .
O7 Mo2 O6 102.0(3) . .
O5 Mo2 O6 88.6(3) . .
O7 Mo2 O12 102.4(3) . .
O5 Mo2 O12 88.6(3) . .
O6 Mo2 O12 155.4(3) . .
O7 Mo2 O8 99.7(3) . .
O5 Mo2 O8 157.4(3) . .
O6 Mo2 O8 86.7(3) . .
O12 Mo2 O8 86.5(2) . .
O7 Mo2 O3 160.5(3) . .
O5 Mo2 O3 64.7(3) . .
O6 Mo2 O3 64.2(3) . .
O12 Mo2 O3 92.7(3) . .
O8 Mo2 O3 93.4(3) . .
O7 Mo2 O4 158.8(3) . .
O5 Mo2 O4 93.8(3) . .
O6 Mo2 O4 91.1(3) . .
O12 Mo2 O4 64.8(3) . .
O8 Mo2 O4 64.2(3) . .
O3 Mo2 O4 40.4(3) . .
O10 Mo3 O11 102.8(3) . .
O10 Mo3 O9 101.3(3) . .
O11 Mo3 O9 155.9(3) . .
O10 Mo3 O8 102.3(3) . .
O11 Mo3 O8 87.8(3) . .
O9 Mo3 O8 87.7(2) . .
O10 Mo3 O13 101.7(3) . .
O11 Mo3 O13 87.9(2) . .
O9 Mo3 O13 86.6(2) . .
O8 Mo3 O13 156.0(3) . .
O10 Mo3 O2 159.4(3) . 7_656
O11 Mo3 O2 64.1(3) . 7_656
O9 Mo3 O2 92.5(3) . 7_656
O8 Mo3 O2 93.4(3) . 7_656
O13 Mo3 O2 63.6(3) . 7_656
O10 Mo3 O4 160.8(3) . .
O11 Mo3 O4 91.2(3) . .
O9 Mo3 O4 65.6(3) . .
O8 Mo3 O4 64.7(3) . .
O13 Mo3 O4 91.7(3) . .
O2 Mo3 O4 39.7(3) 7_656 .
O22 Mo4 O16 101.8(3) . .
O22 Mo4 O17 102.3(3) . .
O16 Mo4 O17 88.5(2) . .
O22 Mo4 O6 103.0(3) . 7_656
O16 Mo4 O6 155.2(3) . 7_656
O17 Mo4 O6 88.1(3) . 7_656
O22 Mo4 O15 100.0(3) . .
O16 Mo4 O15 87.7(3) . .
O17 Mo4 O15 157.7(3) . .
O6 Mo4 O15 86.2(2) 7_656 .
O22 Mo4 O1 158.4(3) . 7_656
O16 Mo4 O1 62.3(3) . 7_656
O17 Mo4 O1 64.8(3) . 7_656
O6 Mo4 O1 94.1(3) 7_656 7_656
O15 Mo4 O1 94.1(3) . 7_656
O22 Mo4 O3 157.8(3) . 7_656
O16 Mo4 O3 93.5(3) . 7_656
O17 Mo4 O3 94.1(3) . 7_656
O6 Mo4 O3 62.2(3) 7_656 7_656
O15 Mo4 O3 64.2(3) . 7_656
O1 Mo4 O3 43.7(3) 7_656 7_656
O19 Mo5 O18 101.2(3) . .
O19 Mo5 O17 103.3(3) . .
O18 Mo5 O17 89.0(2) . .
O19 Mo5 O11 102.0(3) . 7_656
O18 Mo5 O11 156.8(3) . 7_656
O17 Mo5 O11 87.6(3) . 7_656
O19 Mo5 O20 97.9(3) . .
O18 Mo5 O20 87.7(3) . .
O17 Mo5 O20 158.8(3) . .
O11 Mo5 O20 87.2(2) 7_656 .
O19 Mo5 O1 159.4(3) . 7_656
O18 Mo5 O1 62.6(3) . 7_656
O17 Mo5 O1 65.8(3) . 7_656
O11 Mo5 O1 95.2(3) 7_656 7_656
O20 Mo5 O1 94.2(3) . 7_656
O19 Mo5 O2 156.3(3) . .
O18 Mo5 O2 94.4(3) . .
O17 Mo5 O2 94.6(3) . .
O11 Mo5 O2 63.0(3) 7_656 .
O20 Mo5 O2 64.7(3) . .
O1 Mo5 O2 44.0(3) 7_656 .
O14 Mo6 O13 101.2(3) . .
O14 Mo6 O15 101.2(3) . .
O13 Mo6 O15 89.1(3) . .
O14 Mo6 O20 101.5(3) . 7_656
O13 Mo6 O20 88.6(2) . 7_656
O15 Mo6 O20 157.1(3) . 7_656
O14 Mo6 O5 102.3(3) . 7_656
O13 Mo6 O5 156.4(3) . 7_656
O15 Mo6 O5 87.1(2) . 7_656
O20 Mo6 O5 86.0(3) 7_656 7_656
O14 Mo6 O3 159.3(3) . 7_656
O13 Mo6 O3 94.5(3) . 7_656
O15 Mo6 O3 65.3(3) . 7_656
O20 Mo6 O3 92.2(3) 7_656 7_656
O5 Mo6 O3 62.9(3) 7_656 7_656
O14 Mo6 O2 158.4(3) . 7_656
O13 Mo6 O2 63.3(3) . 7_656
O15 Mo6 O2 93.8(3) . 7_656
O20 Mo6 O2 64.9(3) 7_656 7_656
O5 Mo6 O2 93.7(3) 7_656 7_656
O3 Mo6 O2 42.3(3) 7_656 7_656
N1 C1 C2 122.7(8) . .
N2 C2 C1 119.4(7) . .
N2 C2 C3 118.5(7) . .
C1 C2 C3 122.1(7) . .
N2 C4 C5 124.2(8) . .
N1 C5 C4 117.7(7) . .
N1 C5 C6 120.6(7) . .
C4 C5 C6 121.7(8) . .
N3 C8 C9 118.3(7) . .
N3 C8 C7 118.8(7) . .
C9 C8 C7 122.8(8) . .
N4 C9 C8 123.8(7) . .
N4 C10 C12 120.3(8) . .
N4 C10 C11 118.9(7) . .
C12 C10 C11 120.7(8) . .
N3 C12 C10 121.7(8) . .
C1 N1 C5 119.2(6) . .
C1 N1 Cu1 117.7(5) . .
C5 N1 Cu1 123.1(5) . .
C2 N2 C4 116.9(7) . .
C2 N2 Cu2 120.3(5) . .
C4 N2 Cu2 122.7(6) . .
C8 N3 C12 118.7(6) . .
C8 N3 Cu2 125.7(6) . .
C12 N3 Cu2 114.9(6) . .
C9 N4 C10 117.0(6) . .
C9 N4 Cu1 123.8(5) . 8_546
C10 N4 Cu1 119.2(5) . 8_546
P1 O1 O4 52.5(4) . 7_656
P1 O1 Mo1 124.9(4) . 7_656
O4 O1 Mo1 72.4(4) 7_656 7_656
P1 O1 Mo5 122.5(5) . 7_656
O4 O1 Mo5 133.6(5) 7_656 7_656
Mo1 O1 Mo5 94.2(3) 7_656 7_656
P1 O1 Mo4 121.8(4) . 7_656
O4 O1 Mo4 132.3(5) 7_656 7_656
Mo1 O1 Mo4 93.3(3) 7_656 7_656
Mo5 O1 Mo4 91.5(3) 7_656 7_656
P1 O2 O4 54.6(4) . 7_656
P1 O2 O3 54.5(4) . .
O4 O2 O3 92.1(6) 7_656 .
P1 O2 Mo3 126.6(4) . 7_656
O4 O2 Mo3 71.9(4) 7_656 7_656
O3 O2 Mo3 135.4(5) . 7_656
P1 O2 Mo5 120.9(5) . .
O4 O2 Mo5 130.8(6) 7_656 .
O3 O2 Mo5 126.6(5) . .
Mo3 O2 Mo5 92.6(3) 7_656 .
P1 O2 Mo6 123.3(5) . 7_656
O4 O2 Mo6 133.9(6) 7_656 7_656
O3 O2 Mo6 68.7(4) . 7_656
Mo3 O2 Mo6 92.5(3) 7_656 7_656
Mo5 O2 Mo6 91.9(3) . 7_656
P1 O3 O4 53.9(4) . .
P1 O3 O2 54.3(4) . .
O4 O3 O2 91.8(6) . .
P1 O3 Mo2 126.2(5) . .
O4 O3 Mo2 72.3(4) . .
O2 O3 Mo2 134.9(5) . .
P1 O3 Mo6 123.3(5) . 7_656
O4 O3 Mo6 135.6(5) . 7_656
O2 O3 Mo6 69.0(4) . 7_656
Mo2 O3 Mo6 93.1(3) . 7_656
P1 O3 Mo4 121.2(4) . 7_656
O4 O3 Mo4 129.8(5) . 7_656
O2 O3 Mo4 127.5(5) . 7_656
Mo2 O3 Mo4 92.4(3) . 7_656
Mo6 O3 Mo4 91.4(3) 7_656 7_656
P1 O4 O2 58.0(4) . 7_656
P1 O4 O3 57.5(4) . .
O2 O4 O3 95.8(6) 7_656 .
P1 O4 O1 57.2(4) . 7_656
O2 O4 O1 93.6(6) 7_656 7_656
O3 O4 O1 92.3(6) . 7_656
P1 O4 Mo3 126.4(5) . .
O2 O4 Mo3 68.4(4) 7_656 .
O3 O4 Mo3 133.2(5) . .
O1 O4 Mo3 130.8(5) 7_656 .
P1 O4 Mo2 124.7(5) . .
O2 O4 Mo2 133.7(6) 7_656 .
O3 O4 Mo2 67.2(4) . .
O1 O4 Mo2 128.2(5) 7_656 .
Mo3 O4 Mo2 91.8(3) . .
Mo2 O5 Mo6 138.5(4) . 7_656
Mo2 O6 Mo4 140.4(4) . 7_656
Mo3 O8 Mo2 138.5(3) . .
Mo3 O9 Mo1 138.8(3) . .
Mo3 O11 Mo5 139.7(3) . 7_656
Mo2 O12 Mo1 140.3(3) . .
Mo6 O13 Mo3 139.7(4) . .
Mo6 O15 Mo4 138.8(4) . .
Mo4 O16 Mo1 140.3(4) . .
Mo4 O17 Mo5 137.4(4) . .
Mo5 O18 Mo1 139.8(4) . .
Mo6 O20 Mo5 138.0(3) 7_656 .
Mo6 O20 Cu1 117.3(3) 7_656 .
Mo5 O20 Cu1 99.0(2) . .
O4 P1 O4 180.0(5) . 7_656
O4 P1 O2 67.4(4) . 7_656
O4 P1 O2 112.6(4) 7_656 7_656
O4 P1 O2 112.6(4) . .
O4 P1 O2 67.4(4) 7_656 .
O2 P1 O2 180.0(6) 7_656 .
O4 P1 O3 111.4(5) . 7_656
O4 P1 O3 68.6(4) 7_656 7_656
O2 P1 O3 71.2(4) 7_656 7_656
O2 P1 O3 108.8(4) . 7_656
O4 P1 O3 68.6(4) . .
O4 P1 O3 111.4(5) 7_656 .
O2 P1 O3 108.8(4) 7_656 .
O2 P1 O3 71.2(4) . .
O3 P1 O3 180.000(2) 7_656 .
O4 P1 O1 70.3(4) . 7_656
O4 P1 O1 109.7(4) 7_656 7_656
O2 P1 O1 107.3(5) 7_656 7_656
O2 P1 O1 72.7(5) . 7_656
O3 P1 O1 73.3(4) 7_656 7_656
O3 P1 O1 106.7(4) . 7_656
O4 P1 O1 109.7(4) . .
O4 P1 O1 70.3(4) 7_656 .
O2 P1 O1 72.7(5) 7_656 .
O2 P1 O1 107.3(5) . .
O3 P1 O1 106.7(4) 7_656 .
O3 P1 O1 73.3(4) . .
O1 P1 O1 180.0(6) 7_656 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 N4 1.914(6) 8_445
Cu1 N1 1.922(6) .
Cu1 O20 2.418(7) .
Cu2 N2 1.916(6) .
Cu2 N3 1.921(6) .
Mo1 O21 1.651(5) .
Mo1 O12 1.898(5) .
Mo1 O16 1.900(6) .
Mo1 O9 1.901(5) .
Mo1 O18 1.912(6) .
Mo1 O1 2.421(8) 7_656
Mo2 O7 1.657(5) .
Mo2 O5 1.884(6) .
Mo2 O6 1.891(6) .
Mo2 O12 1.891(6) .
Mo2 O8 1.936(5) .
Mo2 O3 2.427(8) .
Mo2 O4 2.507(8) .
Mo3 O10 1.667(5) .
Mo3 O11 1.897(6) .
Mo3 O9 1.897(5) .
Mo3 O8 1.907(5) .
Mo3 O13 1.936(5) .
Mo3 O2 2.441(8) 7_656
Mo3 O4 2.497(8) .
Mo4 O22 1.649(5) .
Mo4 O16 1.889(5) .
Mo4 O17 1.890(6) .
Mo4 O6 1.899(6) 7_656
Mo4 O15 1.936(6) .
Mo4 O1 2.481(8) 7_656
Mo4 O3 2.512(9) 7_656
Mo5 O19 1.669(5) .
Mo5 O18 1.877(6) .
Mo5 O17 1.892(6) .
Mo5 O11 1.901(6) 7_656
Mo5 O20 1.927(5) .
Mo5 O1 2.436(9) 7_656
Mo5 O2 2.489(9) .
Mo6 O14 1.657(5) .
Mo6 O13 1.860(5) .
Mo6 O15 1.888(6) .
Mo6 O20 1.906(5) 7_656
Mo6 O5 1.931(6) 7_656
Mo6 O3 2.488(9) 7_656
Mo6 O2 2.492(9) 7_656
C1 N1 1.326(9) .
C1 C2 1.376(10) .
C2 N2 1.336(10) .
C2 C3 1.506(10) .
C4 N2 1.343(9) .
C4 C5 1.372(10) .
C5 N1 1.334(10) .
C5 C6 1.479(10) .
C7 C8 1.487(11) .
C8 N3 1.337(10) .
C8 C9 1.388(10) .
C9 N4 1.332(9) .
C10 N4 1.340(9) .
C10 C12 1.380(11) .
C10 C11 1.498(12) .
C12 N3 1.346(11) .
N4 Cu1 1.914(6) 8_546
O1 P1 1.571(8) .
O1 O4 1.759(11) 7_656
O1 Mo1 2.421(8) 7_656
O1 Mo5 2.436(9) 7_656
O1 Mo4 2.481(8) 7_656
O2 P1 1.542(9) .
O2 O4 1.678(12) 7_656
O2 O3 1.797(12) .
O2 Mo3 2.441(8) 7_656
O2 Mo6 2.492(9) 7_656
O3 P1 1.546(9) .
O3 O4 1.707(12) .
O3 Mo6 2.488(9) 7_656
O3 Mo4 2.512(9) 7_656
O4 P1 1.482(7) .
O4 O2 1.678(12) 7_656
O4 O1 1.759(11) 7_656
O5 Mo6 1.931(6) 7_656
O6 Mo4 1.899(6) 7_656
O11 Mo5 1.901(6) 7_656
O20 Mo6 1.906(5) 7_656
P1 O4 1.482(7) 7_656
P1 O2 1.542(9) 7_656
P1 O3 1.546(9) 7_656
P1 O1 1.571(9) 7_656
